SCUOLA INTERNAZIONALE SUPERIORE DI STUDI AVANZATI INTERNATIONAL SCHOOL FOR ADVANCED STUDIES

**High temperature physics and**

**nanofriction properties of alkali**

**halide surfaces**

### Thesis submitted for the degree of

*Doctor Philosophiæ*

**Candidate**

: **Supervisor**

:
### Tatyana Zykova-Timan

### Erio Tosatti

**Introduction** **1**

**I The thermodynamics of rocksalt surfaces**

**5**

**1 Overview of bulk and surface melting phenomena** **6**

1.1 Definitions: melting, surface melting and nonmelting . . . 7

1.2 Empirical laws of melting and freezing . . . 12

1.3 Ginzburg-Landau (Cahn-Hillard) theory of surface melting . . . 13

1.4 Occurrence and mechanisms of surface melting/nonmelting . . . . 15

1.5 Alkali halides interface properties near the melting point . . . 18

**2 MD calculations and interatomic potentials** **23**
2.1 Simulation methods . . . 23

2.1.1 Ensembles and temperature control . . . 26

2.1.2 Boundary and initial conditions . . . 26

2.1.3 Model potentials for alkali halides . . . 27

2.1.4 Pressure and surface stress calculation . . . 31

2.1.5 Ewald summation . . . 33

2.1.6 Velocity autocorrelation function and effective harmonic ap-proximation . . . 35

2.1.7 Free energy and thermodynamic integration . . . 36

**3 Bulk NaCl properties molecular dynamics simulation** **37**
3.1 Description of solid alkali halides . . . 37

3.2 Bulk liquid NaCl: the structure of the molten salt . . . 42

3.3 Melting point . . . 44

3.4 Alkali halide vapors and sublimation . . . 47

3.5 Summary . . . 49

**4 Alkali halide surfaces** **50**
4.1 Crystalline NaCl(100): a nonmelting anharmonic surface . . . 50

4.2 Solid surface free energy . . . 52

4.2.1 Thermodynamic integration . . . 52

4.2.2 Effective harmonic approximation . . . 55

4.3 The liquid NaCl surface . . . 56

4.4 Liquid Surface Entropy Deficit: incipient molecular order in the liquid surface . . . 59

**5 Simulation of nanodroplet deposition on NaCl(100)** **67**
5.1 Preparing initial configuration . . . 67

5.2 Droplet evolution . . . 70

5.3 Solid-liquid interface free energy . . . 72

5.4 Discussion . . . 72

Conclusions of part I . . . 73

**II Nanofriction at high temperatures**

**75**

6.1 Motivation . . . 76 6.2 Advantages of using hot NaCl(100) as a substrate . . . 77 6.3 Tip implementation . . . 79

**7 Ploughing friction on NaCl(100)** **82**

**8 Wearless sliding friction on NaCl(100)** **91**

8.1 Influence of the pressure produced by tip on NaCl(100) nonmelting 91 8.2 Wearless sliding . . . 91 8.3 Theory of high temperature wearless friction . . . 96 Conclusions of part II . . . 100

**General conclusions** **103**

**Acknowledgements** **106**

**A Numerical integration algorithm in md3** **116**

Surface science is a mature field, where newer and newer experimental tech-niques have had a strong impact over the last three decades, and where many important and deep conceptual problems have been theoretically tackled and solved. Yet, the tools of surface science have just about begun to come of use for the larger class of problems that encompass strongly developing and strongly relevant areas such as nanoscience, adhesion, and friction.

The scope of this thesis is to use the theoretical and computational tools of surface physics and work out with them a case study whose full solution can have an impact in these areas. The case study we have chosen, is that of understanding the nonwetting habit of a certain crystal surface, sodium chloride (100), by its own melt, and to explore its consequences from various viewpoints, particularly in nanofriction. The reasons for this choice are manifold.

First, the nonwetting phenomenology is there, it is not exclusive to NaCl, and
has been left without an explanation for about thirty years from the experiments
of Mutaftschiev’s group [1]. Second, bad wetting of a solid by a liquid involves
poor adhesion, for which there are many typical examples in nature. However,
*there is no immediate understanding for why should a liquid be repelled by its*

*own solid, as is the case here. Third, alkali halides represent a lucky case where*

thanks to the work of many people some 40-50 years ago, the interatomic forces
are very accurately known, a fact which offers a natural line of attack through
classical computer simulation. This would not be available for the other known
cases of bad self-wetting, occurring mostly in metals and in semiconductors.
Fourth, the high temperature behavior of a solid surface, including a full
cal-culation of its temperature dependent free energy and a comparison with that of
the liquid and of the solid-liquid interface has never been available so far, and
here we can just do it. In particular, despite many long standing bulk studies,
*the physics of the molten salt surface has apparently not been addressed *

prop-erly so far and can have surprises in reserve, as it indeed does. Sixth, simulated nanoexperiments can be carried out for this system, such as the deposition of a nonwetting nanodroplet on the hot solid surface, the melting of a nanocube, the scratching of a hot solid surface by a nanotip. These simulated experiments can be as illuminating as the real ones, albeit less difficult.

This thesis is organized into two parts. Here is an outline of the work which forms its body. The starting point of the project was to reproduce a classic ex-periment demonstrating NaCl partial wetting phenomena done by the group of Mutaftschiev [1, 2, 3] some decades ago. Since the substance used in the exper-iment is rather simple and commonly used the project can be considered a case study and can be easily generalized for the whole class of alkali halide materials. In the first part following this brief introduction, I will present the broad theme of surface melting and nonmelting, as examples of different wetting habits of a liquid onto one face of its own crystalline solid. Next, I will briefly review the known phenomenology of NaCl surfaces with clear indications of partial or in-complete wetting. Then I will introduce the thermodynamical and simulation methods, and the Born-Mayer-Huggins-Fumi-Tosi (BMHFT) interatomic poten-tials that I will employ for my theoretical attack to this general problem, and to the case of an alkali halide in particular and its (100) surface. Many delicate points and well known or less well known pitfalls will be dealt with in this section.

Armed with this instruments, I will present extensive simulations of solid bulk NaCl from low temperatures extending until above the melting point, and of liquid NaCl from somewhat below the melting point upwards. Even at the pure bulk level, one finds that there are still new things that emerge here, despite a wealth of existing studies.

Following these two separate bulk studies, I will consider solid-liquid coexis-tence, and from the simulated behavior of the solid-liquid interface I will extract an accurate value of the bulk melting temperature of the BMHFT model, which is found remarkably close to the experimental value of NaCl. At this point I can begin the surface study properly said. I will describe separately solid-vapor and liquid-vapor interfaces and calculate their free energies. I will also present the deposition of a NaCl liquid nanodroplet on solid NaCl(100) directly illustrating partial wetting. Finally I will explain surface nonmelting and overheating and connect it with partial self-wetting by a simple model. I believe that this is the first study of this kind ever done.

The second part of the thesis is dedicated to the newly developing field of nan-otribology. Here I will attempt to apply our present knowledge of the physics of NaCl(100) to the recently revived problems of friction and wear on atomically flat surfaces when brought to very high temperatures. In practice I will discuss our idealized AFM simulations of a tip sliding in contact mode with the high temper-ature surface. Since I was interested to reveal new frictional phenomena near the bulk melting temperature a natural choice was precisely to work with nonmelt-ing surfaces like NaCl(100) which would resist scratchnonmelt-ing and local heatnonmelt-ing by the tip even at high temperatures.

The nanofriction simulations reveal two distinct and opposite phenomena. Deep
*ploughing friction of a sharp tip shows a drop of the frictional force close to T*M,

where the tip wades or skates through the hot solid, accompanied by a small
moving liquid cloud, the furrow behind promptly healing and recrystallizing. At
the opposite limit, the grazing (wearless) friction of a flat tip shows on the
con-trary a sharp surge of the initially weak frictional force as the surface lattice, still
*solid, turns increasingly compliant near T*M. This surge may be understood as

a nanofrictional analogue of the celebrated peak effect of sliding vortices in the mixed state of type II superconductors.

There have been no attempts as yet to conduct real nanofriction experiments on alkali halides—a very popular substrate at room temperature—at these higher temperatures, but I do hope that there will to verify the predictions that result from our work.

The work contained in this thesis has led and is leading to the following publi-cations:

1. T. Zykova-Timan, D. Ceresoli, U. Tartaglino, W. Zaoui-Sekkal and E. Tosatti,

**NaCl droplets on NaCl(100) at the melting point, Surf.Sci. 566-568, 794 (2004).**

*2. T. Zykova-Timan, D. Ceresoli, U. Tartaglino and E. Tosatti,Why alkali halides*

**solid surfaces do not wet by its own melt?, Phys. Rev. Lett. 94, 176105 (2005).**

*3. T. Zykova-Timan, D. Ceresoli, U. Tartaglino and E. Tosatti, NaCl(100) surface:*

*why does it not melt?, Highlights in the quantum theory of condensed matter, a*
*volume in honor of M.P. Tosi, Scuola Normale Superiore di Pisa (2005).*

*4. U. Tartaglino, T. Zykova-Timan, F. Ercolessi and E. Tosatti, Melting and *

*5. U. Tartaglino, T. Zykova-Timan, F. Ercolessi and E. Tosatti, Surfaces, materials*

**and nanosystems near the melting point, J. Mater. Sci. 40, 2141 (2005).**

*6. T. Zykova-Timan, D. Ceresoli, U. Tartaglino and E. Tosatti, Physics of alkali*

*halide solid and liquid surfaces near the melting point, to appear in J.Chem.Phys.*

*7. D. Ceresoli, T. Zykova-Timan and E. Tosatti, Electron-stimulated emission of*

*Na atoms from NaCl nanocube corners, submitted to Surf.Sci.*

*8. T. Zykova-Timan, D. Ceresoli, U. Tartaglino and E. Tosatti, Physics and *

*nanofric-tion of alkali halide surface near the melting point, submitted to Surf. Sci.*

*9. T. Zykova-Timan, D. Ceresoli, and E. Tosatti, Peak effect versus skating in high*

**The thermodynamics of rocksalt**

**surfaces**

**Overview of bulk and surface**

**melting phenomena**

This chapter is a brief general review of
melt-ing, nucleation and accompanying processes
on solid surfaces. Firstly I will briefly
clas-sify the basic phenomena arising at melting
near the interfaces, paying particular attention
to the connection of wetting (nonwetting) and
melting (nonmelting). Secondly I will survey
the principal experiments, basic approximations
and popular theoretical models used to
pre-dict the melting properties in the past and
nowa-days. Then I will proceed describing the
nu-merical simulations which presently offer a
pow-erful tool to study these and other phenomena.
Here I will confine myself mainly to known
*computational simulations of surfaces at high*
*temperatures. Finally I will focus on surface*

*nonmelting and overheating—the main subjects of the current study— and will*

enumerate the various possible mechanisms of the surface nonmelting that can make solid overheating possible. Of course, in this very fast review of surface melting I do not intend to give a complete description of all the overwhelming and complex problems connected with the melting transition, my goal is merely to show a glimpse to the iceberg apex (Fig. 1).

**1.1 Definitions: melting, surface melting and **

**nonmelt-ing**

*In bulk system the melting point T*M of a homogeneous pure solid phase arises

*when the chemical potentials µ(P,T) of solid and liquid states are equal ( Fig. 1.1).*
Below or above the crosspoint of solid and liquid chemical potentials only the

µ_{L}
µ_{S}

**T**

**M**

**T**

**S**

**T**

**G**

### Temperature

**SOLID**

**LIQUID**

### Chemical potential

*Figure 1.1: The solid µS* *and liquid µL*chemical potentials at fixed P versus

tem-perature. The dash lines show the metastable regions. The melting temperature

*T*M *is a crosspoint of two curves. T*S *and T*G are the spinodal points of the solid

and liquid bulk phases correspondingly.

phase which possesses the lowest chemical potential remains stable. The other
*phase can still exist in its metastable state up to a spinodal point T*Sand down to

*a glass temperature T*G. As a result, it should generally be possible to undercool

the high temperature phase, and to overheat the low temperature phase. Periodic heating and cooling through the first order transition should thus generate a full hysteresis cycle.

In melting, this is only half true. Supercooling of the liquid is allowed by the absence of a solid germ; overheating of the solid is prevented by that omnipresent germ, a surface. This observation provides perhaps the first macroscopic hint that

### (

_{,}

### )

### (

_{,}

### )

### (

_{,}

### )

### sublimation line

### evaporation line

### overheating

### melting line

*l(T)*

### supercooling

**C (liquid)**

**A (solid)**

**B (vapor)**

**T**

_{3}

_{3}

**P**

_{3}

_{3}

**T**

_{C}

_{C}

**P**

_{C}

_{C}

**T**

_{W}

_{W}

**T**

_{M}

_{M}

**P**

_{M}

_{M}

### Pressure

### Temperature

**SOLID (A)**

**VAPOR (B)**

**LIQUID (C)**

Figure 1.2: The generic bulk phase diagram in P-T variables for a pure
homoge-neous system with solid, liquid and gas interface. The melting- and
*sublimation-lines meet the evaporation line at the triple point (T*3*, P*3). The extrapolation of

*the melting line ends at the melting point (TM, PM*) at zero pressure. The

*evapo-ration line ends at the critical point (TC, PC*). The inset shows the surface melting

*which may occur at the solid-vapor interface T*W *< T < T*3.

solid surfaces might be already wet somewhat below the bulk melting point. The
starting motivation for a microscopic study of surface melting begins right there.
In order to find out under which conditions surface melting occurs let us consider
*the system near the triple point (Fig. 1.2) where three phases (solid, liquid, gas,*
for a simple material) are in coexistence. If we move along the coexistence line
*(sublimation line) of two phases A (solid) and B (vapor) towards the triple point*
where the phase C (liquid) becomes thermodynamically stable as a bulk phase,
wetting may arise: a thin film of the third phase C may intervene between A

Figure 1.3: Experimental evidence of surface melting of Pb(110): Medium en-ergy ion scattering shows an increasing number of disordered (liquid) layers ap-proaching the melting temperature. From Ref. [4]

and B (Fig. 1.2, inset), even if the triple point is not yet reached. If phase C (the liquid) wets the A-B interface, a thin wetting film of C can appear well below

*T*M*. The temperature T*Wwhere this process happens is called the surface melting

*temperature or wetting temperature. Surface melting (SM) arises above T*W when

*the thickness `(T ) of the liquid film diverges as T approaches the triple point*
along the sublimation line. SM is quite common for most elemental materials. A
rather famous microscopic characterization of SM is that of Pb(110), first reported
by Frenken and van der Veen [4]. Medium energy ion scattering data revealed
(Fig. 1.3) the presence at the solid-vapor interface of a disordered (liquid) film
*whose thickness `(T ) grows without limit as T → T*M.

SM is not universal, and several surfaces are known that do not melt, but
*re-main solid and crystalline all the way up to T*M. Not surprisingly, this behavior

NM can both occur for the same substance, of course on two different crystal-lographic faces. For example, NM was demonstrated for Pb(111) [6], while by contrast SM prevails on Pb(110).

Exchanging roles of A, B and C we might instead take A = liquid, B = vapor,
C = solid, consider cooling a liquid-vapor interface along the coexistence line,
and ask whether a thin solid film might occur at this interface, above the freezing
*point. This is called surface freezing [7]. In general one can notice a kind of *
symme-try between SM and surface freezing. The SM and the lack of overheating have
been discussed above. Surface freezing of a liquid will similarly imply a lack of
supercooling of the bulk liquid. Surface freezing is a relatively rare phenomenon
characterized by the existence of finite solid surface film floating on the liquid
*phase above T*M. It has been mainly observed in alkanes [8, 9] and alcohols[10].

Clearly SM excludes the possibility of surface overheating and surface freezing
of the liquid excludes the supercooling. The Table.1.1 summarizes the conditions
*of both surface phenomena. In this table γ*SV*, γ*SL*, γ*LV indicate regular interface

*T ≤ T*M *T > T*M

In liquids: bulk supercooling OR surf. freezing

*γ*LV*< γ*SV*+ γ*SL *γ*LV+ *≥ γ*SV*+ γ*SL

In solids: surf. melting OR bulk overheating

*γ*+

SV*≥ γ*LV*+ γ*SL *γ*SV*< γ*LV*+ γ*SL

Table 1.1: Surface phenomena and thermodynamical conditions for their
*exis-tence below and above T*M.

*free energies, whereas γ*_{SV}+ *and γ*_{LV}+ indicate some kind of saddle-point solid-vapor
and liquid-vapor surface free energies, evaluated in a situation where these two
interfaces are not really stable.

In the language of wetting, SM is nothing else than complete interfacial
*wet-ting of the solid by its own melt. ( This is reminiscent, but not really coincident*
*with triple point complete wetting which happens when the solid substrate and the*
wetting liquid are made of different materials)[11]. By contrast, NM corresponds
to partial wetting, schematized in Fig. 1.4. In this case, there is a clear connection
between the surface thermodynamic parameters and the angles of partial
wet-ting [12] as will be clarified further below. Thermodynamically, NM will take
place whenever the solid surface (solid-vapor interface) is unable to lower its free
energy by turning into a sequence of two separate solid-liquid plus liquid-vapor

### solid

### liquid

### γ

_{lv}

### sl

### γ

### γ

### sv

### θ

### lv

### sl

### θ

Figure 1.4: Partial wetting of a solid by its own melt is an indirect evidence of
*surface nonmelting. The γ*LV*, γ*SV *and γ*SL are the free energies of the interfaces;

*θ*SL*and θ*LV are the interior and outer contact angles.

interfaces, namely when

*γ*SV*< γ*SL*+ γ*LV*,* (1.1)

*In general, γ*SV *is at most equal to γ*LV*+ γ*SL*, and γ*LV *is at most equal to γ*SV+

*γ*SL [13]. Conversely, when the inequality (1.1) does not hold, SM will ensue

instead of NM. There is an interesting connection between these interface free energies and the physics of surface melting.

As Fig. 1.3 shows, in SM the liquid film, although technically of divergent
*thick-ness at T*M*, remains atomically thin until fractions of a degree below T*M.

Inter-actions propagate readily across such a thin liquid film. The solid-liquid and the
liquid-vapor interfaces “feel” their mutual presence, so much that they actually
*merge when `(T ) is small enough. For a generic temperature T < T*M the free

*energy change caused by melting a film of thickness ` can be written*

*∆G/A = [(γ*SL*+ γ*LV*) − γ*SV*] + `Lρ*L*(T*M*− T ) + V (`)* (1.2)

*where A is the surface area, L is the latent heat of melting per unit mass, ρ*L is

*the density of the liquid, and V (`) represents a phenomenological “interaction”*
free energy term between the liquid-vapor and the solid-liquid interfaces. As
*defined by (1.2), the interaction V (`) vanishes for ` → ∞, and tends to V (0) =*

*γ*SV*− (γ*SL*+ γ*LV*) when ` → 0, where the dry solid surface free energy is *

*recov-ered. Eq. (1.1) amounts to say that in SM the interface interaction V (`) is globally*

*repulsive, whereas in NM it is attractive. In case when the interactions V (`) *

*be-tween SL and LV are Van der Waals type it takes the form −H/`*2 _{where H is}

Hamaker constant [14].

The microscopic mechanism behind interface attraction or repulsion varies, and may be eventually related to such different physical causes as layering

or-der [12], van or-der Waals forces [15], or molecular oror-der [16]. We will discuss this in detail in Section 1.4.

**1.2 Empirical laws of melting and freezing**

Although in general the melting and freezing transition of a substance is very spe-cific and non-universal, some useful phenomenological criteria have been given to the melting of a solid or the freezing of a liquid which are usually based on the properties of only one of the two coexisting phases. The advantage of these empirical rules is that they sometimes permit a prediction of the solid-liquid co-existence point avoiding much more difficult but more satisfactory free energy calculation.

Two very different rules have been identified. The first starts from the solid phase and the second from the liquid one.

*• The solid-based empirical rule of bulk melting is the so-called Lindemann*

criterion according to which a crystal melts when the amplitude of thermal
vibrations (r.m.s.) reaches a certain percentage of the average size of the
*unit cells [17]. For many materials this Lindemann ratio (∆r*2_{)}*1/2 _{/a is of}*

*order of ' 0.15%. It becomes a useful criterion for melting with a rather*
wide applicability, since the precise value of ratio is insensitive to details
of the potential, at least for simple substances. A generalized formulation
of Lindemann criterion was formulated by Ross [18]. The Ross criterion is
equivalent to assuming the reduced free volume constant along the melting
line. The rule proves quite successful in predicting the melting properties
both of rare gases and liquid metals, given reasonable choices for the pair
potentials.

Atoms at surfaces are less coordinated and more free than in bulk, and
con-sequently their vibration amplitudes are larger. Surfaces may thus reach the
Lindemann instability vibration amplitude at a lower temperature than the
bulk. A model embodying the bulk Lindemann criterion is the
mechani-cal thermal instability model [19]. An infinite solid will, if prevented from
melting, become mechanically unstable at a sufficiently high temperature.
Although the ideal mechanical instability temperature of a solid is different,
*and of course higher than the true melting temperature T*M (where the free

nonetheless heuristically be taken as a qualitative indicator of the tendency
of the solid to melt. Adopting that line, one can ask whether the stability
*of the surface will not cease before that of the bulk. In a model semi-infinite*
solid it is found indeed that the mechanical instability of the first surface
layer occurs at a temperature which is only 73% that of the bulk [20]. This
suggests – correctly – that solid surfaces should begin to soften and melt at
about 3/4 the bulk melting temperature. That is indeed generally the case,
as has been long known and noted by such precursors as Tammann and
Stranski [21]. Self-consistent surface phonon calculations [22] and also
ex-periments [23] in fact reveal a much more pronounced anharmonic outward
expansion of the first surface layer relative to that of the bulk, exhibiting a
*very steep increase well below the melting temperature T*Mof the bulk.

Al-though it is not really possible to generalize, that is undoubtedly one of the qualitative elements heralding a stronger tendency of a surface to become unstable before the bulk.

*• A second liquid-based criterion was formulated by Hansen and Verlet [24].*

For a Lennard-Jones (LJ) liquid they found by computer simulation that the
*first maximum of the liquid structure factor S(k) has a constant amplitude*
of 2.85 along the freezing line. By scattering experiment and by computer
simulation of various systems other than LJ it was found that the maximum
*of S(k) is always close to 3 at freezing. In general the freezing sets in if*
the short-range order in the liquid system, measured by the first maximum
exceeds a certain universal value.

**1.3 Ginzburg-Landau (Cahn-Hillard) theory of surface**

**melting**

To a first approximation, one may consider that liquid and solid differ in their
*(average) density ρ. The simplest theory of SM is based on optimizing the order*
*parameter spatial profile, in particular the density profile ρ(z) of a solid-vapor*
interface in a system with short range interactions. Assuming a bulk grand
*po-tential density ω = ω(ρ), the solid vapor coexistence near the triple point as in*
Fig. 1.2 implies two equivalent solid and vapor minima of the grand potential
*per unit volume ω(ρ) = ωo* plus one additional secondary liquid minimum with

inhomo-T_{M}
S
L
V log∆
ο
(1 − T / )
∆ ∼
ρ
**V**
ρ
ρ
ρ
∆
ρ
ω
ω
z z
SOLID
LIQUID
VAPOR

### (a)

### (b)

### (c)

VAPOR LIQUID SOLID

Figure 1.5: (a) Grand potential profile close to the melting point (solid) and well
*below T*M(dashed) , (b) Mechanical equivalent of the interface free energy

mini-mization (see text), (c) Density profile, showing that the SV interface has split into
*a SL plus LV close to T*M*(solid) but not well below T*M(dashed).

geneous system such as the solid-vapor interface can be written
Ω =
Z Z Z
*d*3* _{x}*
·

*ω(ρ(x)) +*

*J*2

*|∇ρ|*2 ¸ (1.3) In this Ginzburg-Landau (or Cahn-Hillard) type of free energy (acceptable for a system with short range forces) the first term represents the thermodynamic potential density for a uniform system, while the gradient term signifies the extra cost caused by any spatial change in the order parameter (supposed to be slowly

*varying). To describe a solid-vapor interface [25] we may assume ρ = ρ(z) and*seek to minimize Ω (per unit area):

*Ω/A =*
Z
*dz ω(ρ(z)) +* *J*
2
µ
*dρ*
*dz*
¶_{2}
= min (1.4)

*where J > 0 is a parameter, and the constraints ρ(−∞) = ρ*S *and ρ(+∞) = ρ*L,

*where ρ*S*and ρ*V*are solid and vapor densities respectively. ω(ρ(z)) has the shape*

shown on Fig. 1.5a.

This minimum problem is formally identical to the minimum action problem
for the one dimensional Lagrangian motion of a classical point object of
*coor-dinate ρ, mass J, as a function of time z, in a potential V = −ω(ρ) (Fig. 1.5b):*
*Starting at time z = −∞ with zero kinetic energy and with a small ρ = ρ*Vfrom a

*first hilltop of height −ω(ρ*V*) = −ωo* (the vapor phase), the point moves

*“down-hill” eventually reaching at time z = +∞ the last, and exactly equivalent, hilltop*

At temperatures well below the melting point, there is no liquid phase (not
*even metastable), meaning that there exists no liquid-like local minimum in ω(ρ)*
*(Fig. 1.5a, dashed line). Thus −ω(ρ) has no other maxima than the vapor and*
solid hilltops, and the resulting solid-vapor interface is unsplit and featureless
*(Fig. 1.5c, dashed line). Closer to T*M *however −ω(ρ*V) develops a secondary

*maximum—a lower hilltop, as it were—at an intermediate ρ = ρ*L. En route

between the vapor to the solid hilltops, the point particle must negotiate this
intermediate “mountain pass”, where it will not stop, but will still slow down
*considerably. It is easy to check that if ∆ = ω(ρ*L*) − ω(ρ*S) is the height difference

between main and secondary hilltop (the free energy difference between solid
*and liquid, that goes to zero only at the melting point), then the ”time” δz the*
*point will spend near the liquid hill (and therefore with ρ ≈ ρ*Lis proportional to

log ∆). The interface density profile is now split into two interfaces: first a
vapor-liquid one, then a vapor-liquid-solid one (Fig.1.5c). They are separated by a vapor-liquid film
*of density close to ρ*L*, whose thickness ` = δz is logarithmically increasing as*

*T → T*M. And this is just surface melting.

*The above also suggests that one might identify the temperature T∗* _{< T}

M

*where the bulk free energy first develops the local minimum corresponding to*
the liquid phase, with the temperature where a solid surface is likely to begin
wetting itself with the thinnest liquid film. It must be underlined that this simple
heuristic theory only describes SM and cannot account for NM or for many other
complications, upon which we shall return below.

**1.4 Occurrence and mechanisms of surface melting/nonmelting**

Surface melting has been studied in a variety of systems by experiments and by simulations:

**Rare gas solids are reasonably described through a Lennard-Jones potential. As**

first shown by extensive MD studies by Broughton and collaborators [26, 27] they are expected to display surface melting on all crystalline faces. Here truly microscopic experiments are not abundant, because of technical diffi-culties. There is however a large body of work by the surface adsorption community, interested in understanding absorbtion isotherms (a relation-ship between the partial pressure of an adsorbate gas and the surface cov-erage of the adsorbent at constant temperature) as a function of

tempera-ture [28].

**Metals and their surface melting behavior has received by comparison much**

more experimental attention. Metal surfaces usually possess positive Hamaker
constants (see Section 1.1), and generally melt. In detail, they may
occa-sionally exhibit nonmelting, depending on the metal and on the
crystallo-graphic orientation. A minority of close packed surfaces such as Pb(111) [6],
Al(111) and Al(100) [29], etc. display NM, and remain in fact smooth and
*dry all the way to T*M. The vast majority of metal faces consisting of all

other orientations, where packing is poorer, undergo SM. In intermediate
packing cases like for instance Pb(100) [4], the first few layers melt, but the
wetting does not proceed and the liquid film growth is blocked to a finite
*thickness until T*M(incomplete SM). Although this incomplete melting will

macroscopically appear just the same as NM—namely partial wetting with
a finite wetting angle—there is a clear microscopic difference because the
*surface is no longer dry below T*M. An early review of SM on metals can be

found elsewhere [30].

*In surface NM there exists a critical liquid nucleation thickness `crit* which

*is finite above T*M and only vanishes at some “surface spinodal

*tempera-ture” T*SS *> T*M. This fact, first discovered in simulation[5], indicates that in

NM the solid surface is metastable, and protected by a nucleation barrier,
*between T*M*and T*SS. An immediate consequence is that NM solid surfaces

*can be overheated, of course only for a short time, up to at most T*S. For the

(111) surfaces of Pb, Al and Au the calculated amount of maximum
*theo-retical surface overheating O = T*SS*− T*M*is 120K, 150K, and ∼ 150K *

respec-tively. This possibility was demonstrated experimentally by laser heating techniques [31], and also in small Pb clusters [32].

A second interesting point is the microscopic investigation and clarification of the relationship between solid surface NM and its partial wetting by a drop of melt. While macroscopic partial wetting with a nonzero contact angle of the liquid with its own solid is not commonly reported, it is very clearly found by simulation [12].

In addition to the above thermodynamics, there is a simple microscopic
un-derstanding for the physics that leads to NM of the close packed metal
sur-faces. It has to do with the intrinsic atomic structure of the two SL and LV
*interfaces involved. A series of z-resolved in-plane averaged density *
pro-files of the SL and LV interfaces as displayed by MD simulations of suitably

prepared liquid films on Au(111), Au(110), and LJ(111) near their respective

*T = T*M is shown in Fig. 1.6. A well defined damped density oscillation

Figure 1.6: Typical solid-liquid-vapor density profiles obtained by simulations
of Lennard-Jones(110), (111) and Au(110) (three surfaces that undergo SM) just
*below T*M. For Au(111) (which is instead a NM surface) a nonequilibrium

config-uration is shown with two facing equal-period density oscillations which lead to attraction and eventually to the collapse of the two interfaces (see text). Picture from Ref. [33]

is seen to propagate from the solid into the liquid, carrying approximately
the solid interplanar distance as a wavelength. That wavelength of course
depends on the crystallographic direction, in the present example it is large
for (111) but small for (110). A second damped density oscillation starts at
*the liquid surface, carrying inwards a generally different wavelength, *
*deter-mined this time by the main peak in the liquid structure factor S(k). This*
second oscillation (layering), essentially non-existent in the LJ liquid, is

gen-erally strong in a metal. Being a property of the liquid, the surface layering
*oscillation of the surface melted film is obviously face independent.*

When, as in Au(110), the solid and liquid oscillations facing one another possess wavelengths that are out of tune, then their superposition is unfa-vorable and causes interface repulsion, eventually leading to SM. That is what happens most commonly. When instead ( as in Au(111)) the two os-cillations are close to being perfectly tuned, their superposition is favorable and causes interface attraction, leading to NM. This situation is typically realized on the closest packed metal surfaces such as Pb(111), Al(111). Fi-nally, the practical absence of a layering oscillation in the LJ liquid surface indicates indifference of the two interfaces. They nonetheless eventually in-teract via the positive Hamaker constant (see Section 1.1), and therefore SM ensues in that case too.

**Valence semiconductors such as Si, Ge, GaAs and semimetals like Ga are known**

to turn both fully metallic, and denser, either at high pressure or when
they melt at high temperature. This case is special since the van der Waals
forces [13] are inverted in this case, turning the interaction from repulsive to
attractive. In fact, the higher liquid density here causes the Hamaker
*con-stant H to be negative [34], and this necessarily hinders complete surface*
melting. Reports of regular SM with unlimited growth of the liquid film at

*T*Mthat have appeared for Ga [35] are apparently incompatible with the

neg-ative Hamaker constant, and might be an artifact, possibly due to strains.
Due to the long range attraction, regular and complete SM is excluded for
*all faces of these H < 0 materials.*

**1.5 Alkali halides interface properties near the **

**melt-ing point**

Surfaces of ionic crystals such as NaCl, MgO, etc, are often used as substrates for growing other materials, and their properties are therefore better known far below the melting point. Yet, some data are also available about their behavior at

*T*M. As it was discussed long ago in the literature, an ionic salt does not possess

any stable surface that is not neutral[36]. The basic neutral surface is rocksalt structure is 100 (see Fig. 1.7). This surface was well characterized by the neutron scattering [37, 38]. The surfaces of molten salts has been poorly studied so far

Figure 1.7: The fcc crystal structure of NaCl and (100) face

though there are results for surface tension[39], theoretical approaches and early simulations[40].

**The contact angle measurements at the NaCl(100) crystal-melt interface**

Here I will consider the wetting of solid NaCl by its own liquid. A very precise experimental determination of the wettability of NaCl crystal by its own melt was performed by a group of Mutaftschiev beginning in 1975 [1, 2, 3].

Commonly measurements of the crystal-melt contact angle meet great
difficul-ties due to the impossibility of maintaining thermal equilibrium at the melting
point. The widespread method based on the profile of a sessile drop on a solid
*substrate is not an exception. Mutaftschiev et al implemented a new technique*
(so-called ”bubble method”) using inert bubbles injected toward a solid surface
in contact with the melt in a nearly two-dimensional setup. The main advantage
is the possibility to obtain a quasiequilibrium steady state growth solid-melt
*in-terface at a temperature slightly away from T*M. The ultra-pure gas of the bubble

contains fewer impurities with respect to the ambient gas phase during sessile drop observation. It is easy to extract the contact angle at the solid-liquid-vapor interface from the two-dimensional bubble’s profile [41].

The results revealed a surprising lack of complete wetting of the molten salt
on the solid (100) surface, with a large partial self-wetting angle of about 48*◦*

wet-

### θ

### NaCl melt

### NaCl Crystal

### Ar bubble

### A

### B

Figure 1.8: Argon bubble studies of liquid NaCl in contact with the solid revealed a surprising lack of complete wetting, with a large partial wetting angle of about 48 degrees.

*ting angle at T*M is a universal characteristic of the solid-melt contact. It reflects

the interface free energies balance and the nature of the interaction between
*SL-LV interfaces. Mutaftschiev made an attempt at estimating the γ*LV*, γ*SV *and γ*SL

individual contributions[3]. Whereas the contact angle and liquid-vapor free
*en-ergy γ*LV are available from direct measurements of the bubble and of the liquid

*surface tension respectively, the γ*SV*could be only crudely extrapolated from γ*LV

experimental values. That is a bad approximation especially in view of the strik-ing diversity of solid and liquid alkali halide. The last unknown strik-ingredient is

*γ*SL. For many elements it might be indirectly estimated empirically by using e.g.

*Turnbull’s rule [42] which connects γ*SLwith heat of fusion or it could be extracted

from the nucleation experiment [43]. For NaCl(100)/NaCl melt the interface free
*energy γ*SLis simply not known.

In this theoretical thesis I will arrive at reasonably accurate interface free
*ener-gies γ*SV*,γ*LV*, γ*SL*using a specific technique for each of them. γ*LVin particular will

*be derived via a surface stress calculation, γ*SV by a free energy thermodynamic

*integration (the first to our knowledge for a solid surface) and γ*SLis derived from

direct simulation of partial wetting of NaCl(100) by a liquid droplet and subse-quent use of Young’s equation. The detailed physics behind these three numbers will be my main scope, along with explaining in detail the partial wetting results

*of Mutaftschiev et al.*

**How do the NaCl clusters melt?**

Another area of potential interest is the explanation of equilibrium crystal shapes
of NaCl clusters at high temperatures. As it is shown in the experiments of
Heyraud and M´etois (see Fig.1.9) at 893 K the cluster’s profile remains strictly
*cubic and persists up to the corner rounding temperature T*0 *' 923 K. At T*1= 983 K

the facets are entirely separated by rounded regions[44]. This rounding has an interpretation in terms of surface roughnening[45]. However, the roughening ex-planation does not clarify a possible role of liquid-like mobility so very close to the melting point. The rounded region could in reality be a liquid lens, which besides being rough, would also be diffusive and mobile. Alkali halides cluster melting has been addressed by R.S. Berry and collaborators[46], who concluded that melting occurs abruptly. However the role of corners has not yet been inves-tigated properly.

Figure 1.9: The equilibrium crystals of NaCl at (a) 893 K and (b) 983 K. From Ref. [44]

**MD calculations and interatomic**

**potentials**

In present Chapter I will commence with a detailed description of the main tech-nical features used in our Molecular Dynamics (MD) simulations: molecular dy-namics propagators, temperature control, Ewald sum, calculation of pressure and surface tension. Then I will discuss the specific methods applied to the surface such as surface free energy integration, the ”effective” approximation and other necessary techniques used in our study.

**2.1 Simulation methods**

Atomistic simulations constitute a very important tool in the field of melting and surface melting. They can be either of Monte Carlo (MC) type, or of the Molecular Dynamics (MD) type. The main advantage of the MD method over the MC is that it allows the calculation of dynamical properties in addition to the equilibrium properties which can be obtained by either method. Under ”ergodic hypothesis“ one fundamental principle is that ensemble averages can be computed as time averages over the trajectories in the phase space:

*hAi = lim*

*tobs→∞*

Z _{t}_{obs}

0

*A(Γ(t))dt* (2.1)
*where h...i denotes average over ensemble and Γ(t) is the trajectory in phase*
space. The MD simulations consist in solving Newton’s equations of motion

### classical

### empirical

### quantum

### ab initio

### tight−binding

### Potentials:

### comput.cost

### dependability

Figure 2.1: Classification of interatomic potentials.

Figure 2.2: After Ref. [47]

*for all particles of mass Mi*, and coordinates R*i*.

*The basic input needed in MD is the potential energy E*pot*({R}) as a *

func-tion of all coordinates. Depending on systems, and on the accuracy needed, the
choice is between empirical interatomic potentials on one side, and first
*prin-ciples total energy determinations of E*pot*({R}) on the other side. The highest*

physical dependability and computational cost have ”quantum“ interatomic po-tentials which take into account the details of electronic properties of the system, meanwhile the classical interatomic potentials are fitted to certain physical prop-erties (elastic propprop-erties, phononic dispersion curves, etc) and are very effective

for massive calculations. The scheme 2.2 summarizes the potential’s ”hierarchy“
*Next comes the question, how to model E*pot*({R}) in a given specific case*

the interactions between the particles. Empirical two-body potentials, such as Lennard-Jones (LJ), are quite reasonable for rare gas solids or Van der Waals molecular crystals, but not for most other solids. For metals, empirical many body potentials such as the Embedded Atom Model [48], the similar glue model [49], the Finnis-Sinclair potential [50], etc., are much more suitable than two-body forces. Many-body empirical potentials were developed also for such systems as valence semiconductors [51, 52] but here first principles simulations are gener-ally much more appropriate [53].

In practice the integration of Eq.(2.2) is done numerically discretizing time.
Among the possible integration schemes we have implemented the velocity
*Ver-let algorithm, where error in positions is of order O(δt*4_{) and in velocities is of}

*order O(δt*3_{). The method has been shown to have excellent energy-conserving}

properties even with long time steps [54].

The framework of molecular dymanics can be employed for purposes other
than reproducing the time evolution of the system, and computing
thermody-namical averages. Once the forces on the particles are computed, several
”prop-agation“ schemes can be devised: steepest descent, ”smart“ minimization (the
velocities which have opposite signs with forces are nullified), or Langevin
dy-namics [55],etc. For instance, the steepest descent algorithm consists in
*minimiz-ing E*pot*({R}) along a direction of a gradient, once the minimum is reached, the*

gradient is recalculated, a new minimum is sought along the new direction of the gradient. Another application of MD is to find the global minima using the simu-lated annealing technique. The system is initially heated up to high temperatures, then the kinetic energy is gradually removed from the system to reach hopefully the global minimum. The details can be found in Ref. [55]. In some particular simulations we used a damped dynamics at low damping. For these purposes we implemented Ermak’s algorithm for Langevin dynamics [55]. The structure relaxation at 0 K is performed by ”smart minimization“. Further details can be found in Appendix A.

**2.1.1 Ensembles and temperature control**

In the classic MD technique (the simultaneous integration of Newtonian equa-tions of motion) the system total energy is naturally conserved. By maintain-ing the volume constant, the simulation will produce a microcanonical ensemble (NVE), often referred to as Newtonian MD. Other important statistical ensem-bles are the isoenthalpic-isobaric (NPH) developed by Andersen [56], isobaric with variable cell (NPT) in framework of Parrinello-Rahman method [57], and the canonical (isokinetic) (NVT) ensemble. One way to implement the latter is to couple the system to an external thermal bath and control the temperature through the so-called Nos`e-Hoover thermostat [58]. More commonly, the tem-perature control is accomplished simply by velocity-rescaling:

v*new* = v*old*

p

*Tinst/Told* (2.3)

We carried out both microcanonical and canonical simulations. In canonical (NVT) runs, temperature was controlled by velocity-rescaling [59] and only rarely by a Nos`e-Hoover thermostat. We did not resort to (NPT) runs since we deal with surfaces. Moreover our simulations were mainly conducted in the vicinity of melting point where fluctuations become large and isobaric ensemble has much bigger errorbars than the isochoric one.

Despite the size and time limitations imposed by long range forces, great care
was taken to run simulations long enough for a clear equilibration, typically
*100÷300 ps, but longer when required.*

**2.1.2 Boundary and initial conditions**

One of the delicate questions in MD simulations of charged systems are the choice
*of boundary conditions (BC). One can highlight three types: (a) Rigid/fixed BC.*
The boundary atoms coordinates are fixed / the forces acting on them are
nul-lified. It is usually supposed that the number of the fixed atoms is a negligible
fraction of the total system. Therefore the simulation supercell’s size should be
*large. (b) Free BC. The boundary atoms are permitted to move accordingly to*
*their dynamics. In this case the system is treated as a cluster in vacuum. (c) *

*Peri-odic BC. The atoms are placed in periPeri-odically repeated supercell, keeping the total*

The periodic boundary conditions(PBC) exclude the existence of the long wave-length fluctuation (for instance, it is not possible to model the critical point of the liquefied gas) and might have some artificial effects on the dynamics of liquid sys-tems nevertheless it is the best way of modelling the macroscopic bulk syssys-tems with a moderate computational effort.

In our simulations we used periodic boundary conditions(PBC) with minimum
image convention(MIC), i.e. each atom of the ’central’ supercell interacts only
with the closest image of all other particles in neighboring cells. Simulation of
surfaces are commonly done in a slab geometry with periodic boundary
*condi-tions in x, y and free motion along z. In order to minimize spurious slab effects*
at high temperatures, the lateral box size must be adjusted to match the mean
lattice parameter at any desired temperature. The first few bottom layers can be
assumed to be rigid in their bulk-like positions to mimic the contact with a
*semi-infinite slab. In our case, we will repeat slabs periodically along z, separating*
them with a suitable amount of vacuum, as specified later below. In some slab
simulations in order to mimic semi-infinite bulk we have used rigid boundaries.

The velocities initialization is done using the Maxwell-Boltzmann distribution at the desired temperature. The total linear and angular moments are set to zero:

P =
*N*
X
*i*
*mi*v*i* = 0
L =
*N*
X
*i*
*mi*r*i× vi* = 0

The atomic initial positions are randomized from the idealized lattice positions before starting the dynamics to speed up the equilibration process.

**2.1.3 Model potentials for alkali halides**

Alkali halides are among the simplest solids and have been therefore studied for a very long time. Born [60] and followers established quite early that many prop-erties of these crystals could be basically understood by means of simple two-body potentials. The basic ingredients of these potentials are (1) the long-range Coulomb interactions between ions, (2) the short-range repulsion between the ion cores when they get too close. The straightforward implementation of these in-gredients was introduced by Born and Mayer [61]. A significant improvement of the basic model was achieved by Born, Mayer and Huggins [62], who added Van

der Waals and dipole-quadrupole induced terms. All alkali halides were carefully parameterized by Fumi and Tosi [63]. A more realistic but computationally ex-pensive description is done by introducing polarizable potentials that eliminate some of the residual unrealistic features of the rigid ion potentials. There is a vast literature on the bulk properties for solid and liquid alkali halides [64, 65, 66].

In a first approximation alkali halides are two-component mixtures of atomic
anions and cations which interact through a spherically symmetrical potential.
The unusual features of ionic crystals are the infinite range of the potential
inter-actions, which causes the long-range structural correlations, and the strength of
the attractive cation-anion interaction, which cause the presence even in liquids
sharp peaks in the corresponding radial distribution function (i.e. long-lived cage
*structure around each atom). The simplest model for a molten salt is the restricted*

*primitive model, in which ions are modelled by hard spheres, all with the same *

*di-ameter, and with unit positive or negative charges Zi*at the center of each sphere:

*vRP M _{(r}*

*ij*) =

*ZiZj*

*rij*

*+ vHR*

_{(r}*ij*)

*vHR(r) =*(

*∞ (r < σ)*0

*(r ≥ σ)*

The first term is simply a Coulomb potential, the second term is the hard-sphere potential. The RPM model was studied among others by Dietrich [67], Bresme [68] and Fisher [69]. More sophisticated rigid ion models are the Pauling potentials, the (BMH) Fumi-Tosi potentials (see below), the Varshni and Shukla [70] type of potentials.

**Born-Mayer-Huggins rigid ion potentials**

It would be nice to use the best available potentials—those that include polariza-tion effects—for our simulapolariza-tions. However polarizapolariza-tion forces, though not negli-gible for the quantitative description of molecules, low-density ionic fluids, and other properties, appear to be less relevant in the context of the melting transi-tion [71]. This is fortunate, because studies related to melting require simulatransi-tions sizes and times that are difficult to attain with polarizable potentials. Here we adopt the Born-Mayer-Huggins-Fumi-Tosi (BMHFT) model, whose greater sim-plicity allows a much more extensive computational exploration of the melting and wetting properties. Consequently NaCl was modelled by the classic

pair-wise BMHFT rigid ion potential [63]:
*V (rij*) =
*ZαZβ*
*rij*
*+ Aαβexp(−Brij) −*
*Cαβ*
*r*6
*ij*
*−* *Dαβ*
*r*8
*ij*
*.* (2.4)

*The α and β stand for either + or −, Zα* *and Zβ* are the ionic charges (+1 for Na

*and −1 for Cl), the first term is the Coulomb interaction energy, the second is the*
short-range Pauli repulsion, and last two terms are induced dipole-dipole and
dipole-quadrupole van der Waals interactions. The parameters for Na and Cl are
reported in the table 2.1.

Na-Na Cl-Cl Na-Cl
A (eV) 424.097 3488.998 1256.31
B ( ˚A*−1*_{)} _{3.1545} _{3.1545} _{3.1545}

C (eV ˚A6_{)} _{1.05} _{72.5} _{7.0}

D (eV ˚A8_{)} _{0.499} _{145.427} _{8.676}

Table 2.1: Fumi-Tosi parameters of Born-Mayer-Huggins potential for NaCl. From Ref. [66]

**Polarization effects**

Polarization effects are normally incorporated into the simulations of ionic
sys-tems via the shell model. The electron cloud is treated as a spherical shell
con-nected to the center of mass of an ion with a spring. More elaborated models
developed recently employ potentials which include the polarization effects
us-ing either multipole expansions [71] or the distortable ion model [73]. One effect
of ionic polarization in a vibrating crystal is to reduce the splitting of the
longi-tudinal and transverse optic bands. The difference arises from the fact that the
longitudinal and transverse modes give rise to different long-range fields in the
*limit k → 0. In a primitive model of the crystal the LO-TO splitting at the *
Bril-louin zone center obeys by the Lyddane-Sachs-Teller relation:

*ω*2
*LO*
*ω*2
*T O*
= *²*0
*²∞*
(2.5)
*where ωLO* *and ωT O* are the longitudinal and transverse optic mode frequencies

*in the limit k → 0, ²∞*=1 for the rigid ion potentials, whereas for crystalline NaCl

**r (A)**

Figure 2.3: Experimental radial distribution function: g++ (dashed), g*+−*

(solid),g*−−*(dotted) of liquid NaCl. From Ref. [72]

Below we present a brief comparison of calculated surface energies and
relax-ation effects on NaCl(100) obtained within different approximrelax-ations at 0 K (see
Table 2.1.3). One can see in particular that the Fumi-Tosi potential provides a
*good estimation of γ*SValthough the relaxation effects due to the polarization are

absent.

Despite their good quality the main disadvantages of the RPM and rigid ion
potentials are their inability to reproduce dynamical features such as the phonon
dispersion curves in ionic crystals, and the artificial similarity of like pair
dis-tribution functions g*−−* and g++ in fluids absent in experiments (see Fig. 2.1.3).

That may be cured by the implementation the more sophisticated ion potentials calculated from first principles, e.g. shell models or multipole expansion models.

**2.1.4 Pressure and surface stress calculation**

The pressure tensor of a fluid is the negative equilibrium average of the
micro-scopic stress tensor. It is composed of two parts: a kinetic part that arises from
the linear momentum of the molecules and a configurational part that arises from
interatomic forces. The system pressure is calculable through the Clausius virial
theorem:
*pV = NkBT +*
1
3
* * _{N}*
X

*i=1*r

*i· Fi*+ (2.6) (2.7)

*For a pairwise interaction potential U(rij*) the above expression becomes:

*pV = NkBT −*
1
3
*
*N*
X
*i=1*
X
*j>i*
*rij*
*dU(rij*)
*dr*
+
(2.8)
In the case of many-body interactions the pressure profiles can be calculated by a
method of planes [77], or by a modified virial approach [78].

**Surface stress and surface free energy at fluid interfaces**

*The surface excess quantities deal with mechanical equilibrium (balance of forces)*
*and chemical equilibrium (balance of mass transfer) and should be independent*
on the choice of the dividing surface. In this thesis we will often refer to the
*surface tension γ of a homogeneous liquid. Following by Ono and Kondo [79] it*
is useful to review its several determinations (valid for liquids):

**Mechanical:**

*γ =*

Z _{∞}

*−∞*

*(p⊥− p||)dZ*

Physical value BMHFT Madden Ab initio Experiment

*γ*SV(mJ/m2) 191 242 171 *∼276*

∆ Cl-Na ( ˚A) 0.028 0.061 0.0869 0.0874

*Table 2.2: NaCl(100) at 0 K. Our calculation of surface free energy and ∆ = zCl−*

*zN a* buckling, according to ab-initio, BMHFT and polarizable potentials [71, 75]

*where p||and p⊥* are the tangential and normal components of the pressure

*tensor. Isotropy in the xy-plane implies p||* *= px* *= py* *6= p⊥*.

**Statistical:**
*γ = −*1
4
Z _{∞}*−∞*
*dZ*
Z
*d*3** _{r}**X

*αβ*

*x*2

*2*

_{+ y}*2*

_{− 2z}*r*

*fαβ(r)g*(2)

*αβ*

**(r; Z)ρ(Z)***where fαβ(r) is the pairwise force between α and β species at relative *

*posi-tion r. The surface tension evaluaposi-tion in this case completely depends on*
the two body distribution function g(2)_{αβ}**(r, Z) in the interface region.**

**Numerical simulation: Straight implementation for the surface stress **

calcula-tion in MD simulacalcula-tions.
*γ = −* 1
*4LxLy*
*
X
*i,j*
*x*2
*ij* *+ yij*2 *− 2zij*2
*rij*
*f (rij*)
+
(2.9)
*where Lxand Ly* are the in-plane simulation cell sizes.

**Surface stress and surface free energy at solid interfaces**

In contrast to the fluid case, surface free energy and surface stress are not identical
*in solids. The work done dW in creating a new surface dA by applying uniform*
*stress σ on area A is simply*

*dW = σdA = d(γA) = dA(γ +* *∂γ*
*∂AA)*

*where γ is the solid surface free energy. Therefore the thermodynamic relation*
between surface free energy and surface stress per unit area can expressed as:

*σ = γ +* *∂γ*
*∂A*

as first was established by Shuttleworth [80]. Liquids do not support shear, hence
their surface stress is unaffected by any bulk deformations. On the other hand,
solids are rigid and a bulk strain generally changes the surface properties too,
whence *∂γ*

*∂A* *6= 0. As a consequence, all methods given above do not work for a*

solid. As will be explained later, we will recourse to thermodynamical integration
*to calculate γ*SV.

**2.1.5 Ewald summation**

The presence of Coulomb long-range forces severely limits the sizes of our
*sim-ulated systems (upper limit is ∼ 30000 atoms). Since long range forces are *
cru-cial, we rejected the possibility of spherical truncation [81] and implemented the
Ewald summation technique [82]—the most accurate and widely used method
nowadays.

In our case we have an electrically neutral system with a certain distribution of
*point charges qi* in real space. The total charge density can be expressed:

*ρ(r) =*X

n

X

*i*

*qiδ(r − ri− n)*

yielding to the total electrostatic energy

* V (r) =*X
n
X

*i<j*

*qiqj*

*|rij*

*− n|*

*over the simulation cell and its image neighbors, where n = (nxL, nyL, nzL), L*

*is the supercell’s size and nx, ny, nz* are integers. The Ewald summation [83, 54]

method allows to recast Coulomb interactions into two rapidly converging
se-ries: one—in real space and the other—in Fourier(reciprocal) space. In real space
*the point charges qi* are screened by the electrostatic clouds of opposite charge

placed on the ions. The new distribution is short-range rapidly convergent se-ries. In reciprocal space the charged clouds with the same charge as the original point charges are artificially added to compensate the effect of real space electro-static clouds. Finally the self-interaction correction term due to the point charge-compensating cloud repulsion is substracted. The surrounding cloud has a form of a gaussian:

*ρ?(r) = −qi³α*

*π*

´_{3/2}

*e−αr*2 (2.10)

*Parameter α controls the efficiency of the method. The total electrostatic energy*
is given by the following formula:

*V*Ewald**(r) =**
1
*V*
X
*k6=0*
*exp(−k*2* _{/4α}*2

_{)}

*k*2 " X

*j*

*qjexp(−ik · rj*) # " X

*j*

*qjexp(ik · rj*) # + 1

*4π*X

*i*X

*j>i*

*qiqj*

*rij*

*erfc(αrij) −*

*α*

*4π3/2*X

*i*

*q*2

*i*(2.11)

**The first term corresponds to the reciprocal-space summation over k-vectors. The**
*second term is the direct-space summation; erfc(x) is the complementary error*

function:
*erfc(x) = 1 − 2π−*1_{2}
Z * _{x}*
0

*e−t*2

*dt*

The last term represents the self-correction. The scaling with particles number is

*O(N3/2*_{).}

An effective modification of the method is an extensive optimization technique
particle-mesh Ewald (PME) [84]. It developed to perform fast and reliable
simu-lations rely upon an evaluation of the reciprocal-space term using a fast Fourier
transform (FFT). A 3D grid filling the supercell Cartesian space is constructed.
The point ionic charges are interpolated over the grid and the corresponding
*charge distribution ρ(r) is computed. Employing FFT, the transform of the charge*
distribution *ρ(k) is obtained. Next, the long-range contribution of the electro-*ˆ

static potential is estimated ˆ*V (k) = ˆG(k)ˆρ(k) at the various points of the 3D*

grid, where ˆ*G(k) is the so-called influence function defined by ˆG(k) = ˆλ(k)/k*2

*in which λ(r) is a distribution that depends upon the sole geometrical *
charac-teristics of the simulation cell. Electrostatic forces are determined by numerical
derivation of the potential. Finally the electric field and the potential are
interpo-lated back from the grid towards the position of the particles. This scheme has a
*computational effort of O(NlnN ).*

For the slab geometry which we generally use the conventional Ewald
sum-mation technique is not valid anymore since there is no periodicity in one of
*the three dimensions. Parry et al [85] introduced a 2D Ewald summation *
tech-nique(EW2D), whose direct use is found to be computationally expensive [86].
The other algorithms like precalculated tables [87] essentially improve that
per-formance but are not suitable for our type of problem where we need careful
comparison and substraction between bulk and slab systems (see Section 4.2.1).

Another solution is to apply the conventional EW3D to a simulation cell
*elon-gated in z direction so that a sufficiently large empty space between periodic*
*replicas in z is created. The inclusion of empty space between slabs into the unit*
*cell is necessary to avoid an artificial influence from the periodic images in z *
di-rection. Spohr [87] compared the results from the simulations that used EW3D
method with those from the EW2D method. He concluded that the EW3D
con-verges to EW2D when the vacuum thickness in the simulation cell is rather large.
However the correlated fluctuations of surface dipole moment remain important
source of errors.

sum with surface dipole moment correction (EW3DC) *2π*
*3L*3 *|*

P

*iqi*r*i|*

2 _{reduces the}

conventional 3D Ewald sum to the 2D Ewald sum. If the surrounding medium
*has an infinite dielectric constant (ε(ω) = ∞) the surface term vanishes. It is*
equivalent to the “tin foil” or conducting boundary condition. Instead if the
*di-electric constant is finite (ε(ω) = 1 like in vacuum) the surface term becomes *
es-sential and vacuum boundary conditions take place.

In our repeated slab 3D Ewald scheme, a large vacuum thickness of order 100 ˚A separating the slabs is used in order to reduce spurious electrostatic couplings of instantaneous fluctuating dipoles in liquid surfaces facing one another across the vacuum gap. Moreover, we use EW3DC method for better convergence with con-ducting boundary conditions in the tangential directions and with insulating or vacuum boundary conditions in the direction normal to the surface (see Ref. [54]). In development version of the code we have also used PME method [84].

**2.1.6 Velocity autocorrelation function and effective harmonic**

**approximation**

In a solid the main contribution to the entropy comes from the vibrational en-tropy. In bulk as well as in the surfaces the vibrational free energy is of essential importance for phase transitions. It can be calculated approximately within the quasi-harmonic approximation [88] or self-consistent phonon approximation [89, 90]. The harmonic or quasi-harmonic approximations are such that each atom is moving in a parabolic potential well whose curvature is a variational param-eter, calculated variationally with all other atoms rigidly fixed to their mean lat-tice sites. In the self-consistent phonon method the concept is the same, but the parabolic well is calculated by regarding the other atoms as moving. By the Gibbs-Bogoliubov inequality the free energy of the model lattice is always greater than the true free energy but the fitted best parameters are obtained from the min-imum free energy difference. The details can be found in [60].

In our study we needed calculate a surface vibrational entropy of solid NaCl.
*For this purpose we developed a slightly different approach—an effective *
har-monic approximation. Unlike the quasiharhar-monic, or self-consistent harhar-monic
methods, our approach is not self consistent, but uses input from simulations
(Fig. 3.3) that makes it certainly much more accurate. From the simulations we
ex-tracted the vibrational spectrum as the velocity autocorrelation temporal Fourier
*transform [91]. Treating this spectral density D(ω) as a set of the quantum *